3. Results and discussion

#### 3.1. Microstructure

Figure 1(a, b) presents photographs of an as-grown La0.8Sr0.2MnO3 nanowire fabric. The nanowire fabric consists of polymer nanowires containing the ceramic precursor material. The as-grown fabric has a white color, and the entire fabric sample is fully flexible. Figure 1(c, d) finally presents the fully reacted sample after having received the full thermal treatment. The reacted sample shows a fully black color, indicating the completed chemical reaction. As a result, the final nanowire network fabric is extremely thin and brittle. Here, it is important to note that the sample size shrunk to about one sixth of its original size. This shrinkage has to be considered for the application of such fabric-like materials. In the thermal treatment, numerous interconnects between the individual nanowires are formed, which are essential for the

The entire nanowire network was electrically connected by means of silver paint and Cu wires (50 μm diameter) to the sample holder. Due to the high fragility of the ceramic sheet, a pseudo four-point configuration is realized where the current and voltage links connect immediately on the sample contacts. This arrangement is presented in Figure 2. The magnetoresistance is measured in a 10/12 T bath cryostat (Oxford Instruments Teslatron) with a Keithley source meter (model 2400) as a current source, and the voltage is recorded using a Keithley 2001 voltmeter.

Figure 2. Nanowire network sample with electrical contacts for the quasi four-point measurement.

resulting current flow through the sample.

98 Nanowires - Synthesis, Properties and Applications

Scanning electron microscopy revealed an average diameter of the resulting nanowires of around 220 nm and a length of more than 100 μm. Fabric-like nanowire networks with numerous interconnects are formed after the heat treatment. The individual nanowires are polycrystalline with a grain size of about 10–30 nm, which corresponds to the dimensions obtained via transmission electron microscopy and electron backscatter diffraction (EBSD) analysis.

This is presented in Figure 4 giving SEM images of the nanowire network fabrics at 5000 magnification (first column) and at higher magnification (10,000, second column) for all LSMO samples studied here. Figure 4(a) and (b) shows the sample x = 0.2, (c) and (d) the

nanowire. Furthermore, it is obvious from these images that the LSMO grains do not show a

Figure 5. Statistics of the nanowire average grain size (AGS) and the diameter (AD): (a) and (d) La0.8Sr0.2MnO3, (b) and

Magnetoresistance and Structural Characterization of Electrospun La1−*x*Sr*x*MnO3 Nanowire Networks

http://dx.doi.org/10.5772/intechopen.80451

101

Figure 5 presents the detailed analysis of the nanowire diameters and the LSMO grain size determined from several SEM and TEM images. Graphs (a), (b), and (c) show the grain size analysis. The average values were determined using a Gauss fit to the data (indicated by a red line). For the sample x = 0.2, the grain size determined from TEM images varies between 10 and 32 nm with an average of 24.8 nm. Sample x = 0.3 shows grain sizes ranging between 10 and 30 nm with an average of 19.4 nm, and sample x = 0.4 shows an equal distribution of grain sizes with an average grain size of 20 nm. For all samples, the grain sizes determined from the TEM images are larger than the average grain size estimated from XRD, indicating that there are multiply connected domains in the sample. On the sample x = 0.2, we also performed an EBSD analysis of the grain orientations [29], demonstrating the presence of a large number of high-angle grain boundaries within an individual nanowire. The graphs of the nanowire diameters (d, e, f) reveal an average diameter of 227.8 nm for the sample x = 0.2, 251.0 nm for sample x = 0.3, and 223.0 nm for sample x = 0.4. Note that also here the sample x = 0.4 exhibits a

Figure 6 shows finally some high-resolution TEM images of all three LSMO samples studied here. Figure 6(a) and (b) gives grains and their grain boundaries of sample x = 0.2, (c) and (d) images with the same magnification of sample x = 0.3, and (e) and (f) those of sample x = 0.4. For all samples, the LSMO grain size is around 20 nm, and the grains are randomly oriented, resulting in the presence of high-angle grain boundaries between the grains. Furthermore,

texture but are randomly oriented with high-angle grain boundaries between them.

(e) La0.7Sr0.3MnO3, and (c) and (f) La0.6Sr0.4MnO3.

much narrower size spectrum as compared to the other samples studied here.

Figure 4. SEM images of the nanowire network fabrics at 5000 magnification (first column) and at higher magnification (10,000, second column) for all LSMO samples studied here. Images (a) and (b) show the sample x = 0.2, (c) and (d) the sample x = 0.3, and (e) and (f) the sample x = 0.4. The low-magnification images (a, c, and e) present the individual nanowires forming the network fabrics and the numerous interconnects between them. The images with higher resolution (b, d, and f) reveal the polycrystalline structure of the LSMO nanowires. Several small LSMO grains form stacks building up a nanowire.

sample x = 0.3, and (e) and (f) the sample x = 0.4. The low-magnification images (a, c, and e) present the individual nanowires forming the network fabrics and the numerous interconnects between them. These interconnects, formed during the final heat treatment step, are essential for the current flow through the entire sample perimeter and provide additional scattering at their interfaces. The images with higher resolution (b, d, and f) reveal the polycrystalline structure of the LSMO nanowires. Several small LSMO grains form stacks building up a

Magnetoresistance and Structural Characterization of Electrospun La1−*x*Sr*x*MnO3 Nanowire Networks http://dx.doi.org/10.5772/intechopen.80451 101

Figure 5. Statistics of the nanowire average grain size (AGS) and the diameter (AD): (a) and (d) La0.8Sr0.2MnO3, (b) and (e) La0.7Sr0.3MnO3, and (c) and (f) La0.6Sr0.4MnO3.

nanowire. Furthermore, it is obvious from these images that the LSMO grains do not show a texture but are randomly oriented with high-angle grain boundaries between them.

Figure 5 presents the detailed analysis of the nanowire diameters and the LSMO grain size determined from several SEM and TEM images. Graphs (a), (b), and (c) show the grain size analysis. The average values were determined using a Gauss fit to the data (indicated by a red line). For the sample x = 0.2, the grain size determined from TEM images varies between 10 and 32 nm with an average of 24.8 nm. Sample x = 0.3 shows grain sizes ranging between 10 and 30 nm with an average of 19.4 nm, and sample x = 0.4 shows an equal distribution of grain sizes with an average grain size of 20 nm. For all samples, the grain sizes determined from the TEM images are larger than the average grain size estimated from XRD, indicating that there are multiply connected domains in the sample. On the sample x = 0.2, we also performed an EBSD analysis of the grain orientations [29], demonstrating the presence of a large number of high-angle grain boundaries within an individual nanowire. The graphs of the nanowire diameters (d, e, f) reveal an average diameter of 227.8 nm for the sample x = 0.2, 251.0 nm for sample x = 0.3, and 223.0 nm for sample x = 0.4. Note that also here the sample x = 0.4 exhibits a much narrower size spectrum as compared to the other samples studied here.

Figure 6 shows finally some high-resolution TEM images of all three LSMO samples studied here. Figure 6(a) and (b) gives grains and their grain boundaries of sample x = 0.2, (c) and (d) images with the same magnification of sample x = 0.3, and (e) and (f) those of sample x = 0.4. For all samples, the LSMO grain size is around 20 nm, and the grains are randomly oriented, resulting in the presence of high-angle grain boundaries between the grains. Furthermore,

sample x = 0.3, and (e) and (f) the sample x = 0.4. The low-magnification images (a, c, and e) present the individual nanowires forming the network fabrics and the numerous interconnects between them. These interconnects, formed during the final heat treatment step, are essential for the current flow through the entire sample perimeter and provide additional scattering at their interfaces. The images with higher resolution (b, d, and f) reveal the polycrystalline structure of the LSMO nanowires. Several small LSMO grains form stacks building up a

up a nanowire.

100 Nanowires - Synthesis, Properties and Applications

Figure 4. SEM images of the nanowire network fabrics at 5000 magnification (first column) and at higher magnification (10,000, second column) for all LSMO samples studied here. Images (a) and (b) show the sample x = 0.2, (c) and (d) the sample x = 0.3, and (e) and (f) the sample x = 0.4. The low-magnification images (a, c, and e) present the individual nanowires forming the network fabrics and the numerous interconnects between them. The images with higher resolution (b, d, and f) reveal the polycrystalline structure of the LSMO nanowires. Several small LSMO grains form stacks building

Figure 6. High-resolution TEM images with two magnifications of all three types of samples studied here. (a, b) sample x = 0.2, (c, d) sample x = 0.3, and (e, f) sample x = 0.4. The LSMO grains of all samples have sizes of �20 nm, and the grains are randomly oriented with high-angle grain boundaries between them.

bulk materials that the optimized doping level around x = 0.33 supplies the strongest magnetism. The Ms value of all our samples being lower than the bulk values can be attributed to the

Figure 7. M(H) measurement of the LSMO nanowires at T = 10 and 300 K for the LSMO nanowire network fabrics with

Magnetoresistance and Structural Characterization of Electrospun La1−*x*Sr*x*MnO3 Nanowire Networks

http://dx.doi.org/10.5772/intechopen.80451

103

With respect to the literature, the MR data can be divided into two different regimes. According to Ref. [8], the high-field magnetoresistance (HFMR) behavior sheds light on the influence of the sample microstructure via the interface response. Therefore, analyses of the electronic transportation properties and of the magnetoresistive effects of the nanowire networks were carried out by four-probe measurements in external magnetic fields up to 10 T. Firstly, we have a look at the high-field regime. Figure 8 presents the resistance measurements for the samples x = 0.2, 0.3, and 0.4 with the temperature swept from 5 to 300 K. The magnetic field is applied perpendicular to the surface of the nanowire network, i.e., the current flow is mainly perpendicular to the applied field. Magnetoresistance plots are calculated from the data obtained by these sweep measurements at different field strengths using the relation

<sup>M</sup>R %½ �¼ RHð Þ� <sup>T</sup> <sup>R</sup>0ð Þ <sup>T</sup>

As result, we find a maximum MR for the sample x = 0.2 at low temperatures and 10 T applied

<sup>R</sup>0ð Þ <sup>T</sup> : (1)

smaller LSMO grain size of our nanowire network fabric samples.

x = 0.2, 0.3, and 0.4. The insets present the low-field part of the M(H) loops.

3.3. MR data

magnetic field of 70%.

some grain clusters connected with low-angle grain boundaries are also visible, which explains the differences between the grain sizes determined from X-ray data and from TEM images and EBSD [29]. The nanowires are built up from stacks of several individual LSMO grains.

## 3.2. Magnetization data

Figure 7 presents the magnetization data obtained for all three compositions. The soft magnetic character of the LSMO fabric samples is clearly revealed. From the Sr-doping level x = 0.2 to x = 0.4, the saturation magnetization ð Þ Ms is at 10 K 52.12, 58.13, 55.03 emu/g, and at 300 K, and the results are 18.10, 33.09, and 24.62 emu/g, respectively. These values are lower than the ones from the corresponding bulk materials (56 emu/g [30], 33.09 emu/g [31], 24.62 emu/g [32]). The x = 0.3 sample shows the highest Ms among the three compositions, while the x = 0.2 sample shows the lowest ones at both 10 and 300 K. This matches the conclusion drawn from

Magnetoresistance and Structural Characterization of Electrospun La1−*x*Sr*x*MnO3 Nanowire Networks http://dx.doi.org/10.5772/intechopen.80451 103

Figure 7. M(H) measurement of the LSMO nanowires at T = 10 and 300 K for the LSMO nanowire network fabrics with x = 0.2, 0.3, and 0.4. The insets present the low-field part of the M(H) loops.

bulk materials that the optimized doping level around x = 0.33 supplies the strongest magnetism. The Ms value of all our samples being lower than the bulk values can be attributed to the smaller LSMO grain size of our nanowire network fabric samples.

#### 3.3. MR data

some grain clusters connected with low-angle grain boundaries are also visible, which explains the differences between the grain sizes determined from X-ray data and from TEM images and

Figure 6. High-resolution TEM images with two magnifications of all three types of samples studied here. (a, b) sample x = 0.2, (c, d) sample x = 0.3, and (e, f) sample x = 0.4. The LSMO grains of all samples have sizes of �20 nm, and the grains

Figure 7 presents the magnetization data obtained for all three compositions. The soft magnetic character of the LSMO fabric samples is clearly revealed. From the Sr-doping level x = 0.2 to x = 0.4, the saturation magnetization ð Þ Ms is at 10 K 52.12, 58.13, 55.03 emu/g, and at 300 K, and the results are 18.10, 33.09, and 24.62 emu/g, respectively. These values are lower than the ones from the corresponding bulk materials (56 emu/g [30], 33.09 emu/g [31], 24.62 emu/g [32]). The x = 0.3 sample shows the highest Ms among the three compositions, while the x = 0.2 sample shows the lowest ones at both 10 and 300 K. This matches the conclusion drawn from

EBSD [29]. The nanowires are built up from stacks of several individual LSMO grains.

are randomly oriented with high-angle grain boundaries between them.

3.2. Magnetization data

102 Nanowires - Synthesis, Properties and Applications

With respect to the literature, the MR data can be divided into two different regimes. According to Ref. [8], the high-field magnetoresistance (HFMR) behavior sheds light on the influence of the sample microstructure via the interface response. Therefore, analyses of the electronic transportation properties and of the magnetoresistive effects of the nanowire networks were carried out by four-probe measurements in external magnetic fields up to 10 T. Firstly, we have a look at the high-field regime. Figure 8 presents the resistance measurements for the samples x = 0.2, 0.3, and 0.4 with the temperature swept from 5 to 300 K. The magnetic field is applied perpendicular to the surface of the nanowire network, i.e., the current flow is mainly perpendicular to the applied field. Magnetoresistance plots are calculated from the data obtained by these sweep measurements at different field strengths using the relation

$$\text{MR}[\%] = \frac{R\_H(T) - R\_0(T)}{R\_0(T)}.\tag{1}$$

As result, we find a maximum MR for the sample x = 0.2 at low temperatures and 10 T applied magnetic field of 70%.

Table 1 summarizes our findings at three selected magnetic fields for the three doping levels studied here, and the last row of Table 1 gives the maximum MR obtained, together with the

x 100 K 270 K MR max. 0.2 10.24 130 20.66 (22 K) 0.3 6.23 5.98 14.54 (203 K) 0.4 23.58 7.69 26.01 (63 K)

Magnetoresistance and Structural Characterization of Electrospun La1−*x*Sr*x*MnO3 Nanowire Networks

http://dx.doi.org/10.5772/intechopen.80451

105

0.2 27.69 1.81 39 (14 K) 0.3 13.2 6.32 15.18 (169 K) 0.4 17.48 13.00 17.97 (57 K)

0.2 64.12 4.62 69.28 (25 K) 0.3 40.88 5.84 40.93 (92 K) 0.4 41.99 23.47 43.45 (54 K)

Table 1. MR comparison of all LSMO samples measured here at 1, 2.5, and 10 T applied magnetic field.

MR(%) at 2.5 T

MR(%) at 10 T

The last row gives the maximum MR obtained, together with the respective temperature.

At 100 K, sample x = 0.4 shows the highest MR of 23.58% (close to the overall maximum of 26%) at 1 T applied field. In higher applied fields, the maximum value of the MR shifts to sample x = 0.2. A maximum MR ratio of 26.01 at an applied field of 1 T (63 K) is obtained for the sample x = 0.4. At 2.5 T applied field, the maximum MR of 17.97 (57 K) is found in sample

At 10 T applied magnetic field, the maximum MR rate of 69.28% (25 K) is found in sample x = 0.2. Note also that the highest MR of sample x = 0.3 is obtained at a relatively high temperature, ranging from 203 K (1 T) to 92 K (10 T). Secondly, Figure 9 shows the MR ratio of sample x = 0.2 as a function of applied field for various temperatures. The MR is found to increase on lowering the temperature down to 50 K, whereas the MR at low temperature (3 K) is found to be smaller as compared to the 50 K data. The inset of Figure 9 presents the LFMR at an applied magnetic

From the graphs and the tables presented here, three main features can be deduced: Firstly, there is a suppression of the metal-insulator transition. This provides another evidence of the size effect. Nanoscale grains are always accompanied by a large number of grain boundaries, which enhance electron scattering. The metallic behavior is negatively influenced by the Coulomb blockade [13], and as a result, an upturn of the resistivity appears at low temperatures. On the

field of 0.1 T for the sample x = 0.2, showing a maximum LFMR of 5.2% at T = 50 K.

respective temperature.

Doping level MR(%) at 1 T

x = 0.4.

3.4. Discussion

Figure 8. Resistance and MR ratio of all LSMO samples measured up to 10 T applied magnetic field (H⊥sample surface) in the range 2 K < T < 275 K: (a) x = 0.2, (b) x = 0.3, and (c) x = 0.4.


Table 1. MR comparison of all LSMO samples measured here at 1, 2.5, and 10 T applied magnetic field.

Table 1 summarizes our findings at three selected magnetic fields for the three doping levels studied here, and the last row of Table 1 gives the maximum MR obtained, together with the respective temperature.

At 100 K, sample x = 0.4 shows the highest MR of 23.58% (close to the overall maximum of 26%) at 1 T applied field. In higher applied fields, the maximum value of the MR shifts to sample x = 0.2. A maximum MR ratio of 26.01 at an applied field of 1 T (63 K) is obtained for the sample x = 0.4. At 2.5 T applied field, the maximum MR of 17.97 (57 K) is found in sample x = 0.4.

At 10 T applied magnetic field, the maximum MR rate of 69.28% (25 K) is found in sample x = 0.2. Note also that the highest MR of sample x = 0.3 is obtained at a relatively high temperature, ranging from 203 K (1 T) to 92 K (10 T). Secondly, Figure 9 shows the MR ratio of sample x = 0.2 as a function of applied field for various temperatures. The MR is found to increase on lowering the temperature down to 50 K, whereas the MR at low temperature (3 K) is found to be smaller as compared to the 50 K data. The inset of Figure 9 presents the LFMR at an applied magnetic field of 0.1 T for the sample x = 0.2, showing a maximum LFMR of 5.2% at T = 50 K.

#### 3.4. Discussion

Figure 8. Resistance and MR ratio of all LSMO samples measured up to 10 T applied magnetic field (H⊥sample surface)

in the range 2 K < T < 275 K: (a) x = 0.2, (b) x = 0.3, and (c) x = 0.4.

104 Nanowires - Synthesis, Properties and Applications

From the graphs and the tables presented here, three main features can be deduced: Firstly, there is a suppression of the metal-insulator transition. This provides another evidence of the size effect. Nanoscale grains are always accompanied by a large number of grain boundaries, which enhance electron scattering. The metallic behavior is negatively influenced by the Coulomb blockade [13], and as a result, an upturn of the resistivity appears at low temperatures. On the

LFMR on the nanowire diameter, but no information on the LSMO grain size was presented. However, the LFMR at 300 K for our sample is comparable to their data, even though the chemical composition is somewhat different. Nevertheless, this demonstrates that the LFMR as well as the HFMR can be considerably enhanced by reducing the nanowire diameter as well as

Table 2. Magnetoresistance (MR) comparison of different sample types (nanowires, nanoparticles, and powder) of

Magnetoresistance and Structural Characterization of Electrospun La1−*x*Sr*x*MnO3 Nanowire Networks

http://dx.doi.org/10.5772/intechopen.80451

107

Type 100 K 270 K MR max Nanowires [33] 11.2 3.93 20.66 (22 K) Nanoparticles [34] 19.36 4.66 18.7 (79 K) Powder [35] 13.56 6.47 17.66 (50 K)

La0.8Sr0.2MnO3 samples studied in the literature at 1 T applied magnetic field.

Nonwoven nanowire networks of LSMO with three doping levels x = 0.2, 0.3, and 0.4 were fabricated by means of electrospinning. The magnetoresistance effect of these nanowire fabrics was measured up to 10 T applied field between 5 K and 300 K. The reduced dimensions of the nanowires and the large number of interconnects between them were found to increase the MR effect as compared to bulk samples. An MR ratio of 70% was observed for the sample x = 0.2 at

We thank Prof. V. Presser (Saarland University and Institute of New Materials, Saarbrücken) for giving us the possibility to use the electrospinning apparatus. The collaboration Saarbrücken-Nancy was supported by the EU-INTERREG IVa project "GRMN." This work is supported by Volkswagen Foundation and DFG project Ko 2323/8, which is gratefully acknowledged.

, Anjela Koblischka-Veneva1

, Michael R. Koblischka1

\*,

the LSMO grain size.

La0.8Sr0.2MnO3 MR(%) at 1 T

4. Conclusion

Acknowledgements

Author details

Xian Lin Zeng<sup>1</sup>

Jörg Schmauch<sup>1</sup>

low temperatures and 10 T applied magnetic field.

, Thomas Karwoth1

\*Address all correspondence to: m.koblischka@gmail.com

, Uwe Hartmann<sup>1</sup> and Thomas Hauet<sup>2</sup>

1 Institute of Experimental Physics, Saarland University, Saarbrücken, Germany

2 Institut Jean Lamour, UMR CNRS-Université de Lorraine, Vandœvre-lès-Nancy, France

Figure 9. Magnetoresistance of La0.8Sr0.2MnO3 nanowires as function of the applied field for various temperatures. The inset gives the LFMR at 0.1 T applied magnetic field.

other hand, the influence from certain size effects varies with the doping level. So, a step-shape resistance behavior can be observed for the x = 0.2 sample, which indicates that the metalinsulator transition is not completely suppressed. However, in the x = 0.4 sample, the resistance decreases almost linearly from 5 K to 200 K. Secondly, the x = 0.3 sample with the highest saturation magnetization shows the weakest MR effect, and inversely, the x = 0.2 sample exhibits the strongest MR effect at low temperatures. At 2.5 T, the maximum of the MR is already over 40%, which points to an obvious LFMR effect. The increase of the MR with reducing magnetization has been reported by Balcells et al. [8]. In their work, the variation of the grain size is the main reason of the behavior observed. In contrast to this, there is no obvious grain size difference between our samples. The dependence of the MR on the magnetization requires further investigation. Thirdly, at around 200 K with the doping level x = 0.2 and 0.3, the MR curves at 2.5 T have a crossover with the curves at other fields, which means that above 200 K, the absolute value of the magnetoresistance does not monotonously increase with the external field.

To enable a comparison with data on other LSMO sample types but with the same chemical composition (x = 0.2) published in the literature, we summarize some data at 1 T applied magnetic field in Table 2 and compare them with our results.

From Table 2, we see that the nanowire sample x = 0.2 exhibits a larger MR of 20.66% as compared to the nanoparticles and the powder samples of the same chemical composition studied in the literature, however, at some lower temperature. This points clearly to the important contribution of the much smaller LSMO grains in our nanowire network fabric samples, and the additional scattering at the numerous interconnects provides extra MR.

Jugdersuren et al. [19] reported a large LFMR at room temperature in their LSMO nanowires extracted from the networks produced by electrospinning and showed a dependence of the


Table 2. Magnetoresistance (MR) comparison of different sample types (nanowires, nanoparticles, and powder) of La0.8Sr0.2MnO3 samples studied in the literature at 1 T applied magnetic field.

LFMR on the nanowire diameter, but no information on the LSMO grain size was presented. However, the LFMR at 300 K for our sample is comparable to their data, even though the chemical composition is somewhat different. Nevertheless, this demonstrates that the LFMR as well as the HFMR can be considerably enhanced by reducing the nanowire diameter as well as the LSMO grain size.
